Stacking faults and superstructures in a layered brownmillerite
Krüger, H.; Stöber, S.; Welberry, T. R.; Withers, R. L.; Fitz Gerald, J. D.; Acta Crystallographica Section B 67 (2011) 476–485; doi:10.1107/S0108768111042005

data_2105046
_publ_section_title
;
 Stacking faults and superstructures in a layered brownmillerite
;
_journal_coeditor_code           SN5108
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              476
_journal_page_last               485
_journal_paper_doi               10.1107/S0108768111042005
_journal_volume                  67
_journal_year                    2011
_chemical_formula_sum            'Ca4 Fe2 Mn0.5 O9 Ti0.5'
_chemical_formula_weight         467.40
_space_group_IT_number           63
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-A 2a 2a'
_symmetry_space_group_name_H-M   'A m m a'
_audit_creation_method
;
 Jana2000 Version : 18/12/2007
 STOE X-RED
 enCIFer 1.3
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   5.3510(6)
_cell_length_b                   26.669(3)
_cell_length_c                   5.4914(6)
_cell_measurement_reflns_used    2103
_cell_measurement_temperature    298
_cell_measurement_theta_max      29.41
_cell_measurement_theta_min      3.79
_cell_volume                     783.65(15)
_computing_cell_refinement       'STOE X-AREA'
_computing_data_collection       'STOE X-AREA'
_computing_data_reduction        'STOE X-RED'
_computing_molecular_graphics    DRAWxtl
_computing_publication_material
'Jana2000 (Petricek, Dusek & Palatinus, 2000)'
_computing_structure_refinement
'Jana2000 (Petricek, Dusek & Palatinus, 2000)'
_computing_structure_solution
;
 Sir97 (Altomare, A., Burla, M. C., Camalli, M., Cascarano, G., Giacovazzo, C.,
 Guagliardi, A., Moliterni, A. G. G., Polidori, G., Spagna, R., 1997)
;
_diffrn_ambient_temperature      298
_diffrn_detector_area_resol_mean 6.67
_diffrn_measured_fraction_theta_full 0.95
_diffrn_measured_fraction_theta_max 0.95
_diffrn_measurement_device       '2-circle goniometer'
_diffrn_measurement_device_type  'STOE IPDS 2'
_diffrn_measurement_method       'rotation method'
_diffrn_radiation_monochromator  'plane graphite'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0294
_diffrn_reflns_av_sigmaI/netI    0.0046
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       35
_diffrn_reflns_limit_k_min       -35
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_number            3489
_diffrn_reflns_reduction_process
;
 STOE X-AREA/INTEGRATE 1.39
 elliptical profiles, parameters A=15.2,B=2.7,EMS=0.016
;
_diffrn_reflns_theta_full        29.18
_diffrn_reflns_theta_max         29.18
_diffrn_reflns_theta_min         3.79
_exptl_absorpt_coefficient_mu    7.58
_exptl_absorpt_correction_T_max  0.6430
_exptl_absorpt_correction_T_min  0.5289
_exptl_absorpt_correction_type   integration
_exptl_absorpt_process_details
;
 STOE X-RED32 1.31
;
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    3.962
_exptl_crystal_description       block
_exptl_crystal_F_000             912
_exptl_crystal_size_max          0.090
_exptl_crystal_size_mid          0.073
_exptl_crystal_size_min          0.050
_refine_diff_density_max         0.48
_refine_diff_density_min         -0.39
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   2.61
_refine_ls_number_parameters     54
_refine_ls_number_reflns         571
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0253
_refine_ls_R_factor_gt           0.0231
_refine_ls_shift/su_max          0.0002
_refine_ls_shift/su_mean         0.0000
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/(\s^2^(F)+0.0001F^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0330
_refine_ls_wR_factor_ref         0.0336
_reflns_number_gt                543
_reflns_number_total             571
_reflns_threshold_expression     I>3\s(I)
_cod_data_source_file            sn5108.cif
_cod_data_source_block           I
_cod_original_cell_volume        783.64(15)
_cod_original_sg_symbol_Hall     '-A -2xa;-2y;-2za'
_cod_database_code               2105046
_cod_database_fobs_code          2105046